General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.96 - 7.98 g/cm³ Show Material materials with Density of 7.96 - 7.98 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa | |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | ||

100.0 °C | 190 - 194 GPa Show Material materials with Elastic modulus of 190 - 194 GPa | ||

200.0 °C | 182 - 186 GPa Show Material materials with Elastic modulus of 182 - 186 GPa | ||

300.0 °C | 174 - 179 GPa Show Material materials with Elastic modulus of 174 - 179 GPa | ||

400.0 °C | 166 - 172 GPa Show Material materials with Elastic modulus of 166 - 172 GPa | ||

500.0 °C | 158 - 165 GPa Show Material materials with Elastic modulus of 158 - 165 GPa | ||

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | ||

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | ||

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | ||

900.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | ||

1000.0 °C | 120 GPa Show Material materials with Elastic modulus of 120 GPa | ||

Elongation | 20.0 °C | 40 % Show Material materials with Elongation of 40 % | |

Elongation A80 | 20.0 °C | 35 % Show Material materials with Elongation A80 of 35 % | |

Elongation A80, transverse | 20.0 °C | 40 % Show Material materials with Elongation A80, transverse of 40 % | |

Elongation, transverse | 20.0 °C | 30 % Show Material materials with Elongation, transverse of 30 % | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Austenitic Stainless Steel |

Shear modulus | 23.0 °C | 77 GPa Show Material materials with Shear modulus of 77 GPa | Typical for Austenitic Stainless Steel |

Tensile strength | 20.0 °C | 490 - 690 MPa Show Material materials with Tensile strength of 490 - 690 MPa | |

Tensile strength, transverse | 20.0 °C | 490 - 690 MPa Show Material materials with Tensile strength, transverse of 490 - 690 MPa | |

Yield strength Rp0.2 | 20.0 °C | 190 MPa Show Material materials with Yield strength Rp0.2 of 190 MPa | |

50.0 °C | 182 MPa Show Material materials with Yield strength Rp0.2 of 182 MPa | ||

100.0 °C | 166 MPa Show Material materials with Yield strength Rp0.2 of 166 MPa | ||

150.0 °C | 152 MPa Show Material materials with Yield strength Rp0.2 of 152 MPa | ||

200.0 °C | 137 MPa Show Material materials with Yield strength Rp0.2 of 137 MPa | ||

250.0 °C | 127 MPa Show Material materials with Yield strength Rp0.2 of 127 MPa | ||

300.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | ||

350.0 °C | 113 MPa Show Material materials with Yield strength Rp0.2 of 113 MPa | ||

400.0 °C | 108 MPa Show Material materials with Yield strength Rp0.2 of 108 MPa | ||

450.0 °C | 103 MPa Show Material materials with Yield strength Rp0.2 of 103 MPa | ||

500.0 °C | 100 MPa Show Material materials with Yield strength Rp0.2 of 100 MPa | ||

550.0 °C | 98 MPa Show Material materials with Yield strength Rp0.2 of 98 MPa | ||

Unlock all property charts | |||

Yield strength Rp0.2, transverse | 20.0 °C | 190 MPa Show Material materials with Yield strength Rp0.2, transverse of 190 MPa | |

Yield strength Rp1.0 | 20.0 °C | 225 MPa Show Material materials with Yield strength Rp1.0 of 225 MPa | |

50.0 °C | 217 MPa Show Material materials with Yield strength Rp1.0 of 217 MPa | ||

100.0 °C | 199 MPa Show Material materials with Yield strength Rp1.0 of 199 MPa | ||

150.0 °C | 181 MPa Show Material materials with Yield strength Rp1.0 of 181 MPa | ||

200.0 °C | 167 MPa Show Material materials with Yield strength Rp1.0 of 167 MPa | ||

250.0 °C | 157 MPa Show Material materials with Yield strength Rp1.0 of 157 MPa | ||

300.0 °C | 145 MPa Show Material materials with Yield strength Rp1.0 of 145 MPa | ||

350.0 °C | 139 MPa Show Material materials with Yield strength Rp1.0 of 139 MPa | ||

400.0 °C | 135 MPa Show Material materials with Yield strength Rp1.0 of 135 MPa | ||

450.0 °C | 130 MPa Show Material materials with Yield strength Rp1.0 of 130 MPa | ||

500.0 °C | 128 MPa Show Material materials with Yield strength Rp1.0 of 128 MPa | ||

550.0 °C | 127 MPa Show Material materials with Yield strength Rp1.0 of 127 MPa | ||

Unlock all property charts | |||

Yield strength Rp1.0, transverse | 20.0 °C | 225 MPa Show Material materials with Yield strength Rp1.0, transverse of 225 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.65E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.72E-5 - 1.75E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.72E-5 - 1.75E-5 1/K | ||

300.0 °C | 1.75E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.81E-5 - 1.85E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.81E-5 - 1.85E-5 1/K | ||

500.0 °C | 1.84E-5 - 1.85E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.84E-5 - 1.85E-5 1/K | ||

600.0 °C | 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 472 - 500 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 13.3 - 15 W/(m·K) Show Material materials with Thermal conductivity of 13.3 - 15 W/(m·K) | |

100.0 °C | 14.9 W/(m·K) Show Material materials with Thermal conductivity of 14.9 W/(m·K) | ||

200.0 °C | 16.5 W/(m·K) Show Material materials with Thermal conductivity of 16.5 W/(m·K) | ||

300.0 °C | 18.1 W/(m·K) Show Material materials with Thermal conductivity of 18.1 W/(m·K) | ||

400.0 °C | 19.5 W/(m·K) Show Material materials with Thermal conductivity of 19.5 W/(m·K) | ||

500.0 °C | 21 W/(m·K) Show Material materials with Thermal conductivity of 21 W/(m·K) | ||

600.0 °C | 22.4 W/(m·K) Show Material materials with Thermal conductivity of 22.4 W/(m·K) | ||

700.0 °C | 23.8 W/(m·K) Show Material materials with Thermal conductivity of 23.8 W/(m·K) | ||

800.0 °C | 25.2 W/(m·K) Show Material materials with Thermal conductivity of 25.2 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.5 mm²/s Show Material materials with Thermal diffusivity of 3.5 mm²/s | |

100.0 °C | 3.8 mm²/s Show Material materials with Thermal diffusivity of 3.8 mm²/s | ||

200.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

300.0 °C | 4.3 mm²/s Show Material materials with Thermal diffusivity of 4.3 mm²/s | ||

400.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

500.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

600.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

700.0 °C | 5.1 mm²/s Show Material materials with Thermal diffusivity of 5.1 mm²/s | ||

800.0 °C | 5.4 mm²/s Show Material materials with Thermal diffusivity of 5.4 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.5E-7 - 7.91E-7 Ω·m Show Material materials with Electrical resistivity of 7.5E-7 - 7.91E-7 Ω·m |

100.0 °C | 8.45E-7 Ω·m Show Material materials with Electrical resistivity of 8.45E-7 Ω·m | |

200.0 °C | 9.19E-7 Ω·m Show Material materials with Electrical resistivity of 9.19E-7 Ω·m | |

300.0 °C | 9.77E-7 Ω·m Show Material materials with Electrical resistivity of 9.77E-7 Ω·m | |

400.0 °C | 1.03E-6 Ω·m Show Material materials with Electrical resistivity of 1.03E-6 Ω·m | |

500.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

600.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

700.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

800.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.03 % Show Material materials with Carbon of 0.03 % |

Chromium | 16.5 - 18.5 % Show Material materials with Chromium of 16.5 - 18.5 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Molybdenum | 2 - 2.5 % Show Material materials with Molybdenum of 2 - 2.5 % |

Nickel | 10 - 13 % Show Material materials with Nickel of 10 - 13 % |

Nitrogen | 0.11 % Show Material materials with Nitrogen of 0.11 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |